Ceramics International 30 (2004) 1993–1998 Spin, charge, and orbital orderings in oxides with dual-valent transition metal ions R. Vidya∗ , P. Ravindran, P. Vajeeston, H. Fjellvåg, A. Kjekshus Department of Chemistry, University of Oslo, Box 1033 Blindern, N-0315 Oslo, Norway Received 8 November 2003; received in revised form 9 December 2003; accepted 22 December 2003 Available online 2 July 2004 Abstract Using generalized-gradient-corrected full-potential density-functional calculations, we have studied the electronic structure and magnetic properties of YBaMn2 O5 , Sr4 Fe4 O11 , and Ca3 Co2 O6 . In these phases, the 3d transition metal ions have dual valence. We have studied the electronic structure using site-, angular momentum-, and orbital-projected density of states. The charge and orbital ordering are analyzed in terms of the calculated electron-density distribution, charge density, and electron localization function. The oxygen vacancy, cation radii, and crystal-field effects are found to play an important role for the various ordering phenomena in these compounds. © 2004 Elsevier Ltd and Techna Group S.r.l. All rights reserved. Keywords: C. Magnetic properties; D. Transition metal oxides; Spin, charge, and orbital ordering 1. Introduction Since the discovery of colossal magnetoresistance (CMR) in perovskite-like manganites there have been increased activities on related oxides with dual-valent transition metal constituents. Beside the technological interest in the CMR effect, other related phenomena (attractive from more fundamental points of view) have been established for dual-valent compounds. A very interesting phenomenon is the tendency displayed by many transition metal oxides to adopt the kind of charge distribution known as charge ordering (CO). Although covalence effects in such compounds can be significant, the ionic picture describes it as a real-space ordering of charges and/or orbitals. In general, the Coulomb repulsion between the charges and the elastic energy perturbation owing to cooperative Jahn–Teller (JT) distortions favor the CO. Large radius of (what may be conveniently named) A-site cations (RA ) and wide eg bandwidths, favor the mobility of the electrons through the lattice, while smaller RA and narrow eg bandwidths, favor localization . CO is interesting because double-exchange gives rise to metallicity along with ferromagnetism (F) while the CO state can be ∗ Corresponding author. E-mail address: firstname.lastname@example.org (R. Vidya). URL: http://folk.uio.no/ravindrv. associated with insulating and antiferromagnetic (AF) behavior. Hence, there is a competition between F with metallic behavior and insulating AF character with CO. Orbital ordering (OO) gives rise to anisotropic interactions in the electron-transfer process which in turn favor or disfavor the double- and super-exchange (F or AF) interactions in an orbital direction-dependent manner. Understanding of the CO, OO, and spin ordering (SO) processes, provides a foundation for deeper penetration into the complex behaviors of CMR materials. In the present work, we analyze the spin, charge, and orbital orderings present in the dual-valent oxides (with crystal structure more or less related to the perovskite-type) YBaMn2 O5 (YBMO), Sr 4 Fe4 O11 (SFO), and Ca3 Co2 O6 (CCO). We have used full-potential density-functional calculations to understand the electronic and magnetic properties and the various orderings present in these phases. 2. Computational details The full-potential linear muffin-tin orbital (FPLMTO) calculations  presented in this paper are all-electron, and no shape approximation to the charge density or potential has been used. The basis set is comprised of augmented linear muffin-tin orbitals . The calculations 0272-8842/$30.00 © 2004 Elsevier Ltd and Techna Group S.r.l. All rights reserved. doi:10.1016/j.ceramint.2003.12.198 1994 R. Vidya et al. / Ceramics International 30 (2004) 1993–1998 are based on the generalized-gradient-corrected (GGA) density-functional theory as proposed by Perdew et al. . Spin–orbit coupling is included directly in the Hamiltonian matrix elements for the part inside the muffin-tin spheres, hence for spin-polarized cases the size of the secular matrix is doubled. We used a multi-basis in order to ensure well-converged wave functions. This means that several Hankel or Neumann functions, each attached to its own radial function, have been used. The basis included are Y 4p, 5s, 5p, and 4d, Ba 5p, 6s, 6p, 5d, and 4f , Mn 4s, 4p, and 3d, and O 2s, 2p, and 3d for YBMO, Sr 5s, 4p, 4d, and 4f , as well as pseudo-core 5p, Fe 4s, 4p, and 3d, and O 2s, 2p, and 3d for SFO, and Ca 4s, 4p, and 3d, Co 4s, 4p, and 3d, and O 2s, 2p, and 3d for CCO. For the total-energy study the k-space integration is done with 192, 144, and 90 k points for YBMO, SFO, and CCO, respectively, in the irreducible part of the first Brillouin zone. For the magnetic calculations, the easy magnetization axis is chosen in accordance with experimental findings [5–7]. 3. Results and discussion 3.1. YBaMn2 O5 The ordered oxygen-deficient double perovskites RBaT 2 O5 (R = rare-earth and T = Mn, Fe, or Co) have attracted much attention as new spin–charge–orbital coupled CMR materials. CMR effects of some 40% are observed in the isostructural phases with R = Gd or Eu . At low temperature, YBMO is an AF insulator with CO of Mn3+ and Mn2+ accompanied by OO and SO. The crystal structure (Fig. 1) is described in the space group P4/nmm with two kinds of MnO5 pyramids arranged in an ordered manner, each Mn2+ O5 pyramid being linked to five Mn3+ O5 pyramids and vice versa . Oxygen takes two crystallographically different sites with O(1) at the base of the square pyramids, and O(2) at the apex. The basal plane Mn3+ –O(1)–Mn2+ angle is 157.8◦ and the apical Mn3+ –O(2)–Mn2+ angle is 180◦ . The large difference in these angles play a key role in the magnetic properties. Table 1 Calculated magnetic moment (in µB per T atom at 0 K) for YBMO, SFO, and CCO in the ground-state configuration Compound YBaMn2 O5 (YBMO) Sr4 Fe4 O11 (SFO) Ca3 Co2 O6 (CCO) Theory Experiment T(1) T(2) Total T(1) T(2) Total 3.07 2.86 0.17 3.93 3.35 2.63 0.86 0.00 1.21 2.91 0.00 0.08 3.91 3.00 3.00 0.95 0.0 1.3 Total refers to the total magnetic moment per formula unit. The experimental values are taken from Refs. [5–7]. Among the paramagnetic (P), F, and AF configurations considered for calculations , AF is found to have the lowest total energy. The ferromagnetic configuration is 505 meV/f.u. higher in energy than the AF configuration. Table 1 shows that the total magnetic moment is not completely canceled, resulting in a ferrimagnetic (Ferri) state. Mn(1) has a smaller magnetic moment (3.07 µB ) than Mn(2) (3.91 µB ) implying that Mn(1) corresponds to Mn3+ and Mn(2) to Mn2+ , both in high-spin states. The electronic structure indicates that it is an indirect band-gap semiconductor with a band gap of 0.88 eV, in agreement with experimental findings [10,11]. CO is expected to be favored when equal proportions of Mn2+ and Mn3+ are present like in YBMO. On reduction of the Mn–O–Mn angle, the hopping between the Mn 3d and O 2p orbitals decreases and hence the eg bandwidth decreases. Consequently the system stabilizes in a Ferri-CO-insulating state. In order to visualize the presence of CO and Ferri SO in YBMO we show the calculated d-electron-density distribution for the Mn ions in the up- and down-spin channels in Fig. 1a and b. The CO in YBMO is characterized by the real-space ordering of Mn2+ and Mn3+ . The significant difference in the electron-density distribution for the Mn ions clearly indicates that there occurs two different valence states with different orbital occupation. This feature ensures that the spins do not cancel exactly, resulting in the Ferri ordering (Fig. 1c). The exchange interaction between Mn2+ and Mn3+ along c is AF owing to the 180◦ bond angle which facilitates p–d bonding with the O(2) pz orbital as well Fig. 1. The calculated Mn d-electron-density distribution of (a) up- and (b) down-spin electrons in YBaMn2 O5 . (c) The G-type ferrimagnetic spin ordering and (d) orbital ordering in YBaMn2 O5 . R. Vidya et al. / Ceramics International 30 (2004) 1993–1998 as super-exchange interaction . With a bond angle of only 157◦ within the basal plane, the d(Mn)–p(O) covalent bond is weak and moreover due to the HS state of Mn3+ in the square-pyramidal crystal field, the dx2 −y2 orbital at the Mn3+ site is almost empty whereas that at Mn2+ is half filled. Hence, the AF super-exchange interaction between Mn2+ and Mn3+ within the basal plane is weaker than that along c. In order to visualize the OO in YBMO we show in Fig. 1d the electrons distribution at the Mn sites between −1 eV and EF (viz. the electrons mainly participating in the hopping interactions). In the bc plane the dz2 orbital is ordered along c for both Mn3+ and Mn2+ , and this orbital hybridizes with the O(1) pz orbital resulting in bonding. There is virtually no overlap between the dx2 −y2 and pz orbitals because of their different orientation in the c direction. Therefore, the electron in the dx2 −y2 orbital can not hop along c. Moreover, the direct overlap between O px,y and Mn d is small in the ab plane (dx2 −y2 is almost empty for Mn3+ and only partly occupied for Mn2+ due to the JT distortion) and hence the d electrons become localized resulting in CO and OO. 3.2. Sr 4 Fe4 O11 SFO is also an oxygen-deficient perovskite-like material which crystallizes in the space group Cmmm . It is an antiferromagnet with TN ≈ 230 K. Fe has square-pyramidal [Fe(1)] and octahedral [Fe(2)] coordination polyhedra. Owing to the oxygen vacancy in the structure and different crystal-field effects Fe takes the dual-valent states Fe3+ and Fe4+ . According to powder neutron diffraction data (at 8 K) this compound has an unusual magnetic structure; Fe(1) do not exhibit any magnetic ordering whereas Fe(2) ions have a G-type AF arrangement . The room-temperature Mössbauer spectrum is reported  to show two symmetrical doublets of equal intensity. From the isomer-shift values (0.35 and −0.08 mm s−1 ) the two components are assigned to Fe3+ and Fe4+ . A hyperfine splitting and low flux density value has been observed for the Fe3+ component, whereas only a linewidth broadening is observed for the Fe4+ component below TN . This suggests a partially frustrated AF structure . Furthermore, a strong divergence between zero-field-cooled and field-cooled magnetic susceptibility curves is observed, implying spin-glass-like behavior . We have carried out density-functional calculations in F as well as A-, C-, and G-type AF configurations and found that G-AF has the lowest energy. C-AF is the next stable state with 2.54 eV higher energy than the G-AF state. Our calculations show that G-AF configuration with zero magnetic moment for Fe(1) is higher in energy (1.85 eV) than that with a magnetic moment of 2.8 µB for Fe(1), indicating that the former may represent a meta-stable state. However, we have not considered temperature effects and oxygen vacancy ordering in our calculations which may play important 1995 roles for the magnetic properties. The unusual magnetic properties of SFO can be related to the crystal structure and the CO of the Fe ions. In order to be able to draw a more firm conclusion regarding the magnetic structure, further calculations including structural optimization is in progress. A correct assignment of valence states to the Fe ions is essential to understand the relationship between the crystal structure and the electronic and magnetic properties. The Mössbauer studies appear to point to the presence of Fe3+ and Fe4+ ions. Crystal-field stabilization energy and the relative values of the bond-strength sums  indicate that Fe4+ should be assigned to square-pyramidal and Fe3+ to octahedral coordinations. If Fe(1) were an Fe4+ ion, it 4 e0 ; 2 µ ) should be either in an intermediate-spin (IS; t2g B g 4 e0 ; 0 µ ) state. The octahedral state or in a low-spin (LS; t2g B g 4 e1 ; 3 µ ). An IS state for Fe(2) should be Fe3+ in IS (t2g B g Fe(2) agrees very well with the theoretical and experimental magnetic moment and is consistent with the JT distortion observed. The electronic structure of SFO in the G-AF state is consistent with metallic conductivity with a low density of states (DOS) at the Fermi level (EF ). The partial DOS analysis shows that the Fe 3d and O 2p states are energetically degenerate leading to covalent interaction between them. However, as the topology of the DOS curves for Fe(1) and Fe(2) is different (Fig. 2), the magnitude of the covalent interaction is also different. In the G-AF state with the zero magnetic moment for Fe(1), the up- and down-spin DOS of Fe(1) are similar, implying that the up- and down-spin channels have the same occupancy, viz. complying with the zero magnetic moment. This emphasizes the fact that Fe(1) exists in an Fe4+ LS state. The majority spin channel of Fe(2) has more states than the minority spin channel, giving a finite magnetic moment (also seen for Fe(1) in the G-AF situation where Fe(1) takes a finite magnetic moment). As the Fe(2)–O bond length (2.04 Å) is longer than the Fe(1)–O bond length (1.85 Å), the Fe(2)–O bond strength is weaker than that of Fe(1)–O. On the other hand, more unpaired 3d states are localized on Fe(2) than on Fe(1). Moreover, as the Fe(1)–O–Fe(2) bond angle is less than 180◦ , the super-exchange interaction is incomplete like the Mn(1)–O–Mn(2) super-exchange interaction in YBMO. These features lead to the CO in addition to the SO in SFO. 3.3. Ca3 Co2 O6 CCO belongs to the family of one-dimensional (1-D) oxides. Inorganic structures with 1-D atomic arrangements are in the limelight owing to their unique electronic and magnetic properties . The crystal structure of CCO consists of parallel 1-D Co–O chains separated by Ca2+ ions. The chains are built by alternating face-sharing CoO6 octahedra and trigonal prisms along the hexagonal c axis. The resulting short metal–metal intrachain distance (2.59 Å) (compared to the interchain distance of 5.24 Å) reinforces the 1-D character of the structure along the c axis. Mag- 1996 R. Vidya et al. / Ceramics International 30 (2004) 1993–1998 Fig. 2. The site- and angular momentum-projected density of states for Fe(1) and Fe(2) of Sr 4 Fe4 O11 . The s and p partial DOSs are only about 10% of the d states shown. netic studies show F intrachain ordering (TC1 = 24 K) with AF interchain coupling (TC2 = 10 K) . For every two F-aligned Co chains, there is one AF-aligned chain giving a resultant Ferri structure. Our total-energy study  shows that Ferri state of CCO has the lowest energy in perfect agreement with experimental findings [6,18]. The Ferri state is 114 meV/f.u. lower in energy than the F state. The electronic structure shows  a finite DOS at EF in both spin channels, implying a metallic character consistent with the experimental conductivity study . Our partial DOS analysis shows that the states in the vicinity of EF are mainly contributed by Co d states. Different spin configurations for the crystallographically different Co ions are expected  as a consequence of the larger crystal field for the octahedral Co(1) than for the trigonal prismatic Co(2). Various proposals have been made for spin states of Co such as (i) Co(1): LS Co3+ ; Co(2): HS Co3+ , (ii) Co(1): LS Co4+ ; Co(2): HS Co2+ , and (iii) Co(1): LS Co2+ and Co4+ ; Co(2): HS Co3+ . The calcu- lated magnetic moments listed in Table 1 are found to be in good agreement with available low-temperature neutron diffraction and magnetization data. By taking the magnetic moments at the Co sites into consideration, together with the octahedral and trigonal-prismatic crystal fields and the calculated site- and orbital-projected DOS features, we con5 e0 ) state and Co(2) clude that Co(1) is Co4+ in LS (d 5 ; t2g g 5 e2 ) state. is Co2+ in HS (d 7 ; t2g g As the interatomic distance in metallic Co is 2.51 Å and the distance between Co(1) and Co(2) in CCO is 2.59 Å, a metallic interaction between Co(1) and Co(2) has been anticipated . However, our charge density and electron-localization-function analyses show very weak metallic interaction between the Co atoms. Moreover as seen from Fig. 3, the topology of DOS curves for Co(1) and Co(2) are entirely different implying differences in their valence and spin states. As the O 2p states are energetically degenerate with Co 3d states, there is strong covalent R. Vidya et al. / Ceramics International 30 (2004) 1993–1998 1997 Fig. 3. The site- and angular momentum-projected density of states for Co(1) and Co(2) of Ca3 Co2 O6 . The Co s and p partial DOSs are only about 10% of the d states shown. interaction between Co and O. However, the magnitude of covalent interaction is different for Co(1) and Co(2) owing to the difference in their crystal fields. Therefore, the localization of charges on Co(1) and Co(2) is different and leads to the ladder-type CO. Moreover, the orbital-projected DOS features show that both eg and t2g (except dxz ) orbitals have finite states close to EF for Co(1) whereas only dxz and dyz orbitals have finite DOS in the same region for Co(2). Therefore, also the occupation of the d orbitals of Co(1) and Co(2) is different resulting in OO in addition to the CO and Ferri-SO situation. ordering. The occupancy of the d orbitals and hence orbital ordering is determined by the coordination polyhedra surrounding the T ions. Therefore, the crystal-field effect and hence crystal structure of a compound play an important role in orbital ordering. All in all, the constituents of a given compound, the crystal structure (including crystal-field effects), and oxygen stoichiometry determine spin, charge, and orbital orderings in this type of materials. A study of the individual effect of the just mentioned ruling parameters may reveal more insight into the ordering phenomena. Acknowledgements 4. Conclusions We have studied the electronic and magnetic properties (in particular spin, charge, and orbital orderings) of YBMO, SFO, and CCO, using full-potential density-functional calculations. All the studied compounds have dual-valent transition metal ions which (together with at least two crystallographically non-equivalent T -atom sites) is a prerequisite for the ordering phenomena under investigation. The present study, however, shows that the phenomena are not connected to one particular structure type. In general, when the eg bandwidth (determined mainly by the constituents of the compound) is small, charge ordering is favored. In YBMO, the distinction between the radii of Y and Ba together with oxygen vacancies (not discussed here) lead to difference in T (1)–O–T (2) bond angles as well as T –O bond lengths. Hence the T (1)–O–T (2) super-exchange interaction is not uniform in YBMO resulting in a charge ordering pattern of the checker-board type. Similarly, in SFO and CCO also the variation in the bond angles and bond lengths leads to difference in the valence states of the T ions and charge The authors are grateful to the Research Council of Norway for financial support. Part of these calculations were carried out on the Norwegian supercomputer facilities. References  C.N.R. Rao, A.K. Raychaudhuri, in: C.N.R. Rao, B. Raveau (Eds.), Colossal Magnetoresistance, Charge Ordering and Related Properties of Manganese Oxides, World Scientific, Singapore, 1998, p. 31.  J.M. Wills, O. Eriksson, M. Alouani, D.L. Price, in: H. Dreysse (Ed.), Electronic Structure and Physical Properties of Materials, Springer, Berlin, 2000, p. 148.  O.K. Andersen, Phys. Rev. B 12 (1975) 3060.  J.P. Perdew, K. Burke, M. Ernzerhof, Phys. Rev. Lett. 77 (1996) 3865.  F. Millange, E. Suard, V. Caignaert, B. Raveau, Mater. Res. Bull. 34 (1999) 1.  S. Aasland, H. Fjellvåg, B.C. Hauback, Solid State Commun. 101 (1997) 187.  H. Fjellvåg, unpublished. 1998 R. Vidya et al. / Ceramics International 30 (2004) 1993–1998  C. Martin, A. Maignan, D. Pelloquin, N. Nguyen, B. Raveau, Appl. Phys. Lett. 71 (1997) 1421.  R. Vidya, P. Ravindran, A. Kjekshus, H. Fjellvåg, Phys. Rev. B 65 (2002) 144422.  J.P. Chapman, J.P. Attfield, M. Mölgg, C.M. Friend, T.M. Beales, Angew. Chem. Int. Ed. Engl. 35 (1996) 2482.  T.P. Beales, M. Mölgg, J. Jutson, C.M. Friend, Phys. Stat. Sol. (A) 161 (1997) 271.  J.B. Goodenough, Magnetism and the Chemical Bond, Wiley, New York, 1963.  J.P. Hodges, S. Short, J.D. Jorgensen, X. Xiong, B. Dabrowski, S.M. Mini, C.W. Kimball, J. Solid State Chem. 151 (2000) 190.  L. Fournes, Y. Potin, J.-C. Grenier, G. Damazeau, M. Pouchard, Solid State Commun. 62 (1987) 239.  T.C. Gibb, J. Chem. Soc., Dalton Trans. (1985) 1455.  T.N. Nguyen, H.-C. zur Loye, J. Solid State Chem. 117 (1995) 300.  R. Vidya, P. Ravindran, H. Fjellvåg, A. Kjekshus, O. Eriksson, Phys. Rev. Lett. 91 (2003) 186404.  H. Kageyama, K. Yoshimura, K. Kosuge, X. Xu, S. Kawano, J. Phys. Soc. Jpn. 67 (1998) 357.  A. Maignan, C. Michel, A.C. Masset, C. Martin, B. Raveau, Eur. Phys. J. B 15 (2000) 657.  H. Kageyama, K. Yoshimura, K. Kosuge, H. Mitamura, T. Goto, J. Phys. Soc. Jpn. 66 (1997) 1607.  H. Fjellvåg, E. Gulbrandsen, S. Aasland, A. Olsen, B.C. Hauback, J. Solid State Chem. 124 (1996) 190.